VIEWS: 16 PAGES: 25 POSTED ON: 5/25/2011
NASA/CR-2002-211758 ICASE Report No. 2002-25 An Irreversible Constitutive Law for Modeling the Delamination Process Using Interface Elements Vinay K. Goyal and Eric R. Johnson Virginia Polytechnic Institute and State University, Blacksburg, Virginia Carlos G. Dávila NASA Langley Research Center, Hampton, Virginia Navin Jaunky ICASE, Hampton, Virginia August 2002 The NASA STI Program Office . . . in Profile Since its founding, NASA has been dedicated • CONFERENCE PUBLICATIONS. to the advancement of aeronautics and space Collected papers from scientific and science. The NASA Scientific and Technical technical conferences, symposia, Information (STI) Program Office plays a key seminars, or other meetings sponsored or part in helping NASA maintain this cosponsored by NASA. important role. • SPECIAL PUBLICATION. Scientific, The NASA STI Program Office is operated by technical, or historical information from Langley Research Center, the lead center for NASA programs, projects, and missions, NASA’s scientific and technical information. often concerned with subjects having The NASA STI Program Office provides substantial public interest. access to the NASA STI Database, the largest collection of aeronautical and space science STI in the world. The Program Office • TECHNICAL TRANSLATION. English- is also NASA’s institutional mechanism for language translations of foreign scientific disseminating the results of its research and and technical material pertinent to development activities. These results are NASA’s mission. published by NASA in the NASA STI Report Series, which includes the following report Specialized services that complement the types: STI Program Office’s diverse offerings include creating custom thesauri, building customized • TECHNICAL PUBLICATION. Reports of data bases, organizing and publishing completed research or a major significant research results . . . even providing videos. phase of research that present the results of NASA programs and include extensive For more information about the NASA STI data or theoretical analysis. Includes Program Office, see the following: compilations of significant scientific and technical data and information deemed to be of continuing reference value. NASA’s • Access the NASA STI Program Home counterpart of peer-reviewed formal Page at http://www.sti.nasa.gov professional papers, but having less stringent limitations on manuscript • Email your question via the Internet to length and extent of graphic help@sti.nasa.gov presentations. • Fax your question to the NASA STI • TECHNICAL MEMORANDUM. Help Desk at (301) 621-0134 Scientific and technical findings that are preliminary or of specialized interest, e.g., quick release reports, working • Telephone the NASA STI Help Desk at papers, and bibliographies that contain (301) 621-0390 minimal annotation. Does not contain extensive analysis. • Write to: NASA STI Help Desk • CONTRACTOR REPORT. Scientific and NASA Center for AeroSpace Information technical findings by NASA-sponsored 7121 Standard Drive contractors and grantees. Hanover, MD 21076-1320 NASA/CR-2002-211758 NASA/CR-2000- ICASE Report No. 2002-25 An Irreversible Constitutive Law for Modeling the Delamination Process Using Interface Elements Vinay K. Goyal and Eric R. Johnson Virginia Polytechnic Institute and State University, Blacksburg, Virginia Carlos G. Dávila NASA Langley Research Center, Hampton, Virginia Navin Jaunky ICASE, Hampton, Virginia ICASE NASA Langley Research Center Hampton, Virginia Operated by Universities Space Research Association Prepared for Langley Research Center under Contract NAS1-97046 August 2002 Available from the following: NASA Center for AeroSpace Information (CASI) National Technical Information Service (NTIS) 7121 Standard Drive 5285 Port Royal Road Hanover, MD 21076-1320 Springfield, VA 22161-2171 (301) 621-0390 (703) 487-4650 AN IRREVERSIBLE CONSTITUTIVE LAW FOR MODELING THE DELAMINATION PROCESS USING INTERFACE ELEMENTS VINAY K. GOYAL∗ , ERIC R. JOHNSON† , CARLOS G. DAVILA‡ , AND NAVIN JAUNKY§ ´ Abstract. An irreversible constitutive law is postulated for the formulation of interface elements to predict initiation and progression of delamination in composite structures. An exponential function is used for the constitutive law such that it satisﬁes a multi-axial stress criterion for the onset of delamination, and satisﬁes a mixed mode fracture criterion for the progression of delamination. A damage parameter is included to prevent the restoration of the previous cohesive state between the interfacial surfaces. To demonstrate the irreversibility capability of the constitutive law, steady-state crack growth is simulated for quasi-static loading-unloading cycle of various fracture test specimens. Key words. composite structures, progressive failure, ply damage mode, intradamage mode, interlami- nar damage mode, delamination, interface elements, decohesion elements, buckling, postbuckling Subject classiﬁcation. Structural Mechanics 1. Introduction. Delamination in composite structures usually originates from geometric discontinu- ities and material defects such as free edges, dropped plies, re-entrant corners, notches, and transverse matrix cracks. Recently, signiﬁcant progress has been made in the development of tools to predict intralaminar dam- age, which often precedes the onset of delamination. Delamination can be a major failure mode in composites structures and can lead to signiﬁcant loss of structural integrity. Fracture mechanics techniques such as the virtual crack closure technique (VCCT)[1, 2] has been successfully used in the prediction of delamination growth. However, an initial delaminated area must be predeﬁned and a self-similar crack growth is assumed. To overcome the limitations associated with the VCCT, interface elements can be located between composite lamina to simulate initiation of delamination and non-self-similar growth of delamination cracks without specifying an initial crack. Delamination is initiated when the interlaminar traction attains the maximum interfacial strength, and the delamination front is advanced when the local surface fracture energy is consumed. A softening constitutive law that relates tractions to the relative displacements is generally used to formulate interface elements. The softening constitutive law is based on the procedures used by Dugdale[3] and Barenblatt[4] to ﬁnd the extent of the plastic zone ahead of the crack tip in ductile metals; the size of which is chosen such that the stress singularity from linear elastic fracture mechanics disappears. The softening portion of the constitutive law accounts for the complex mechanisms occurring in the volume of material ahead of the crack tip by which large amounts of energy are absorbed in the fracture process. For laminated composites these mechanisms include nucleation, growth and coalescence of microcavities. Hilleborg[5] developed the ﬁrst comprehensive interface ﬁnite element model and applied this method in ∗ Graduate Research Assistant, Aerospace and Ocean Engineering Department, Virginia Polytechnic Institute and State University, Blacksburg, VA 24061-0203 † Professor, Aerospace and Ocean Engineering Department, Virginia Polytechnic Institute and State University, Blacksburg, VA 24061-0203 ‡ Aerospace Engineer, Analytical and Computational Methods Branch, NASA Langley Research Center, Hampton, VA 23681-2199 § Senior Staﬀ Scientist, ICASE, NASA Langley Research Center, Hampton, VA 23681-2199. This research work was supported by NASA Langley Research Center under NASA Contract No. NAS1-97046 while in residence at ICASE, NASA Langley Research Center, Hampton, VA 23681-2199. 1 concrete cracking. Later, Needleman[6] developed a cohesive-decohesive formulation to simulate dynamic crack growth in isotropic elastic solids. The exact mathematical form of the interfacial constitutive law is less important than its capability to represent the maximum interfacial strength and critical fracture energy. Hence, the functional dependence of the traction ﬁeld on the displacement jump across the interface is not uniquely deﬁned. However, functions with continuous derivatives have a numerical advantage over functions with discontinuous derivatives when used with Newton-Raphson method because the tangent stiﬀness is smooth. A smooth tangent stiﬀness as a function of the relative opening displacement has been found to mitigate the numerical oscillations encountered in using a softening constitutive relation and to eliminate oscillatory convergence diﬃculties[7]. The exponential function for the softening constitutive law is smooth and mimics the physics involved in the separation of two atoms initially bonded[8]. This form of the constitutive law has been used in the analysis of crack initiation, dynamic growth, branching, and arrest in homogeneous materials[9]. Shahwan and Waas[10] used it to study delamination of composite structures caused by compressive loads. The various exponential constitutive laws that have been successfully employed to simulate delamination are based on the assumption that the consumed local surface fracture energy can be recovered. This assumption is invalid for structural systems with stresses that may internally redistribute upon external loading in such a way that cracks arrest and cracks faces close. Ortiz and Pandolﬁ[11] postulated a damage model and used an exponential constitutive law to account for such irreversibilities. A limitation of this model is that the critical energy release rates and the maximum interfacial strengths associated with Mode I, Mode II, and Mode III fracture cannot be speciﬁed separately. The present work aims at the establishment of an exponential softening constitutive law that satisﬁes empirical mixed-mode delamination failure criteria for the onset and progression of delamination. An internal state variable is included in the constitutive law to permanently damage the internal surfaces that have exceeded maximum strength during the deformation process. The paper is structured as follows: (i) mixed- mode fracture criteria, (i) mechanics of idealized interface material, (ii) interface ﬁnite element, (iii) ﬁnite element results, and (iv) concluding remarks. 2. Mixed-Mode Failure Criteria. A quadratic failure criterion based on interlaminar tractions has been used to predict onset of delamination[12, 13]. To simulate the progression of delamination under mixed- mode loading conditions, the power law form of the fracture criterion that includes Mode I, Mode II and Mode a III interaction has been successfully used with a bilinear constitutive law[14, 15, 16]. D´vila and Camanho[17] developed a bilinear constitutive law that can be used with any mixed-mode failure criterion. To the authors’ knowledge, no work has been found incorporating an empirical failure criteria into the exponential softening constitutive law. A brief description of the failure criteria used in this paper is presented next. 2.1. Criterion for the Onset of Delamination. Under pure Mode I, Mode II, or pure Mode III loading, the onset of delamination occurs when the corresponding interlaminar traction exceeds its respective maximum interfacial strength. However, under mixed-mode loading, delamination onset may occur before each traction component reaches its maximum interfacial strength. An expression that considers the inter- action between the traction components under mixed-mode loading is the multi-axial stress criterion given as α α α 1/α ¯ T1 T2 T3 (2.1) Te = c + c + c =1 T1 T2 T3 2 where Tj is the interlaminar traction component associated with the j-direction, Tjc is the maximum in- terlaminar traction, and T3 = T3 , if T3 > 0, otherwise it is zero. This function has been included to emphasize that the normal compressive traction T3 does not contribute to the onset of delamination. In ¯ Equation 2.1, Te is an eﬀective normalized traction, and α ≥ 2 is a real number that determines the shape ¯ ¯ of the tri-dimensional failure surface. Delamination does not initiate if Te < 1, and initiates when Te = 1. With α = 2, one recovers the quadratic delamination interaction. The failure surface for α = 2 is a convex semi-sphere in the space of normalized tractions Tj /Tjc , j = 1, 2, 3. As the value of α is increased, the failure surface approaches a half-cube surface. 2.2. Criterion for Progression of Delamination. Delamination propagates when the energy release rate equals its critical value under pure Mode I, Mode II, or pure Mode III fracture. Generally, delamination growth occurs under mixed-mode loading. Under this type of loading, delamination growth might occur before any of the energy release rate components attains its individual critical value. The power law criterion based on the one proposed by Whitcomb[18] is α/2 α/2 α/2 GI GII GIII (2.2) + + =1 GIc GIIc GIIIc where Gj is the energy release rate under Mode j fracture, and Gjc is the single-mode critical energy release rate for j = I, II, III. The material parameter α deﬁnes the shape of the failure locus. For α = 2, one recovers the linear interaction criterion[19]. The shape of the failure locus is a triangular surface. The shape of the failure surface approaches a 1/8-cube surface as α increases from 2. Reeder[20] evaluated diﬀerent fracture criteria for mixed-mode delamination in a brittle graphite/epoxy composite, a toughened graphite/epoxy composite, and a tough graphite/thermoplastic composite using the mixed-mode bending (MMB) test specimen. The power law criterion was a reasonable ﬁt to the test data for the three diﬀerent materials. Thus, the failure criterion in Equation 2.2 is incorporated into the constitutive law of the interface material. 3. Mechanics of the Idealized Interface Material. The interfacial material is bounded by an upper surface S + and lower surface S − . These surfaces are assumed to coincide with a reference surface S 0 in the undeformed conﬁguration as is shown in Figure 6.1. Thus, it is said that the interface material is of zero thickness. The surfaces S ± independently displace and stretch, and are connected by a continuous distribution of nonlinear springs that act to resist the Mode I opening or Mode II and Mode III sliding of the upper and lower surface. It is convenient to deﬁne a mid-surface S m where the tractions and relative displacements are evaluated. For this purpose, let us consider any two points P + and P − contained in S + and S − , which are coincident in the undeformed conﬁguration. The locus of the midpoints P m of the line joining P + and P − deﬁne the mid-surface S m of the interface material. Refer to Figure 6.2. The normal and tangential components of the traction and relative displacement vector are determined by the local orientation of the mid-surface S m . The virtual work done by the cohesive-decohesive tractions is given by (3.1) δWint = δ j Tj dS m Sm for any kinematically admissible relative displacements j , where Tj are the interlaminar traction compo- nents acting on a unit deformed area conjugate to the relative displacements, and S m is the surface area. The resistive tractions that are associated to the relative displacements at the point P m are shown in Figure 6.2. The interlaminar normal traction is denoted T3 and the tangential tractions are denoted T1 and T2 . 3 In the next section, the components of the relative displacements are obtained in terms of the displace- ment ﬁeld with respect to the undeformed conﬁguration. Next, the constitutive equations that relate the relative displacements to the traction ﬁeld are presented. The kinematics and the constitutive modeling describe the mechanics of interface debonding. 3.1. Kinematics of the Interface Material. The fundamental problem introduced by the interface material is the question of how to express the virtual relative displacements between the surfaces S ± in terms of virtual displacements. As shown in Figure 6.1, consider a three-dimensional space with Cartesian coordinates Xi , i = 1, 2, 3, and let there be surfaces S ± coincident with S 0 deﬁned in this space by Xi = Xi (η1 , η2 ), where η1 , η2 are curvilinear coordinates on the surface S 0 . Let the Cartesian coordinates x± = x± (η1 , η2 ), i = 1, 2, 3 describe motion of the upper and lower surfaces i i S ± in the deformed conﬁguration. Any point on S ± in the deformed conﬁguration is related to the same point on S 0 through (3.2) x± = Xi + Ui± i where Ui± are displacement quantities with respect to the ﬁxed Cartesian coordinate system. The coordinates xm = xm (η1 , η2 ), i = 1, 2, 3 deﬁne the mid-surface S m given by i i 1 + 1 (3.3) xm = i xi + x− = Xi + i U + + Ui− 2 2 i The surface S m is coincident with S 0 in the undeformed conﬁguration. As mentioned earlier, the components of the relative displacement vector are evaluated at the mid-surface S m . Therefore, the local orientation of normal and tangential unit vectors to the surface S m is required. This is, T ∂xm ∂xm ∂xm 1 (3.4) r1 = , 2 , 3 ∂η1 ∂η1 ∂η1 T ∂xm ∂xm ∂xm 1 (3.5) r2 = , 2 , 3 ∂η2 ∂η2 ∂η2 and the normal vector is simply (3.6) r3 = r1 × r2 The tangential vectors r1 , r2 may not be perpendicular in a curvilinear coordinate system so that, (3.7) r2 = r3 × r1 For i = 1, 2, 3, the normal and tangential unit vectors to the surface S m at a point P m ∈ S m are ri (3.8) r ˆi = |ri | These unit vectors deﬁne the local orthogonal coordinate system at S m and are related to the ﬁxed coordinate system through the rotation matrix (3.9) r r r R = [ˆ1 , ˆ2 , ˆ3 ] The normal and tangential components of the relative displacements vector expressed in terms of the dis- placement ﬁeld is, (3.10) i + − = Rji (x+ − x− ) = Rji Uj − Uj j j 4 where Rji are components of the rotation matrix. Since xm depends on the displacements Ui± , the rotation i matrix also depends on Ui± . Therefore, the virtual relative displacement are expressed in terms of the virtual displacements as follows, − − (3.11) δ i = Rji (δUj − δUj ) Equation 3.11 is substituted into Equation 3.1 to obtain the expression of the internal virtual work in terms of the virtual displacements. This form of the internal virtual work is convenient for the ﬁnite element formulation. In addition, the diﬀerential surface area of the mid-surface dS m in the deformed conﬁguration is expressed in the form, (3.12) dS m = M dS 0 where dS 0 is the diﬀerential undeformed surface area, and M is a function of the displacement ﬁeld Ui± . 3.2. Constitutive Equations for the Interface Material. The stress singularities at the crack-tip in the linear elasticity solutions, stemming from the sharp slit approximation, cannot be reconciled with any realistic local rupture process. From the molecular theory of strength it is known that there exists stress limits for which molecular bond rupture occurs. The softening-type of cohesive zone model is intended to represent the degradation of the material ahead of the crack-tip. It captures strength-based bond weakening, and fracture-based bond rupture. The mechanics of the delamination process comprises three interrelated phases: (i) the initiation of delamination, (ii) the evolution of the degradation zone, (iii) and the delamination growth. The ﬁrst phase that takes place is the initiation of delamination, and it is based on a stress limit determined experimentally. A stress measure that is used as the limiting value, may involve an interaction of interlaminar stresses such as that in Equation 2.1. The second event is the development of a zone ahead of the crack-tip that experiences intense deformation such as plastic deformation in metals, elongated voids that contains a ﬁbrous structure bridging the crack faces in polymers (crazing), and high density of tiny cracks in brittle ceramics. The molecular bonds are weakened and the nonlinear softening behavior is conﬁned in this degradation zone, or process zone. The third event, is the growth of delamination, bond-rupture, and it is based on a fracture criteria such as Equation 2.2. The constitutive equations to be developed, mathematically describe these three delamination phases. The focus of this section is to develop the constitutive equation for single-bond rupture based on continuum damage mechanics approach. This particular case is extended to mixed-mode delamination. The constitutive equations that are postulated in this section, are shown to satisfy the failure criteria for initiation and progression of delamination presented in the previous section. Assume that the two material points P + and P − contained in S + and S − as shown in Figure 6.2 are connected with a spring. The points are coincident when the spring is unstretched, and a high initial spring stiﬀness restrains the relative displacement of these material points. Under isothermal conditions, the traction T that acts to resist the relative displacement of these material points is due to stretching of the spring, and is expressed as 1− ¯β (3.13) T ( ) = Tc ¯ exp β c where ¯ = / , and T c is the maximum bonding strength that occurs at the critical stretching value c . The parameter β with β ≥ 1 and β ∈ R+ deﬁnes the stretching range for which the bond is weakened before complete rupture occurs. It is in this range, that damage accumulates. In Figure 6.3, the traction-stretching curve is shown for diﬀerent values of the parameter β. The work of debonding per unit area, Gc , is given by 5 the area under the traction-stretching curve, or, ∞ (3.14) Gc = T ( )d 0 2 1 = Tc c β (2−β)/β Γ exp β β where Γ[z] is the Euler gamma function of argument z. By prescribing T c , Gc , and β in Equation 3.14, the parameter c can be computed. The exponential function in Equation 3.13 is a suitable representation of a softening constitutive law because with increasing stretching of the spring , the traction T increases c to a peak value T and then decreases until complete debonding occurs. Equation 3.13 is only valid for monotonically increasing separation because the work due to stretching is recoverable on unloading. ˜ An internal state variable d that tracks the damage state of the spring needs to be included in Equation 3.13 to account for irreversible eﬀects. In the following irreversible law an elastic damage model instead of a plastic damage model is assumed, 2 − ¯ β /d − d ˜ ˜ (3.15) T ( ) = T c ¯ exp β ˜ Within the framework of continuum damage mechanics, it is possible to impose restrictions on d. It must increase as a function of time because thermodynamics requires that the irreversible dissipation associated ˙ ˜ with the debonding process remains semi-positive, i.e., d ≥ 0. An equivalent mathematical expression at a discrete time ti is (3.16) d(ti ) = max 1, d(ti−1 ) , ¯ β i ) , d(0) = 1 ˜ ˜ (t ˜ with ti > ti−1 . If the spring is assumed undamaged at t = t0 , then the initial condition is d(t0 ) = 1. Equation ˜ 3.15 is equivalent to Equation 3.13 if no damage occurs, d = 1, or for monotonic increasing loading, d = ¯ β . ˜ ˜ (ti ) Unloading does not occur linearly to the origin, but with an exponential form. The energy of dissipation associated to fatigue is neglected in this work. This assumption is valid in the case of a spring that undergoes a small number of loading-unloading cycles. Equations 3.15 and 3.16 with β = 1 are used for the traction-stretching curve shown in Figure 6.4. The points on the curve labeled 1, ..., 6 in this ﬁgure, represent a possible loading-unloading cycle of the spring connecting terminal points P ± . The spring is unstretched at point 1. With increasing stretching cohesive traction develops to resist the separation. Point 2 is in the stiﬀening portion of the constitutive law, and the action of the spring prevents much separation of points P ± . The onset of delamination occurs at point 3, where the traction attains its maximum value. As the spring is stretched beyond the onset of delamination to point 4, damage accumulates in the spring and the traction gradually decreases. Assume unloading commences at point 4, then the spring begins to contract to point 5. If loading commences from point 5, the spring is stretched again to point 6 on the original softening portion of the constitutive law. Continued loading from point 6 is along the original softening portion of the constitutive law. The traction eventually vanishes as the spring is stretched substantially beyond point 6. Equations 3.15 and 3.16 are extended to the mixed-mode delamination case. To develop the constitutive equations, it is convenient to normalize the relative displacements and the tractions Tj with respect to j c the critical separation values j and the maximum interfacial strengths Tjc . That is, c (3.17) ¯j = j/ j, Tj = Tj /Tjc ¯ 6 In reference to Figure 6.2, the components of the normalized relative displacements between P ± with respect to the orientation of the surface S m at a point P m is, (3.18) v = ¯ 1 ˆ1 + ¯ 2 ˆ2 + ¯ 3 ˆ3 r r r where ˆ1 , ˆ2 , ˆ3 are the unit vectors tangent and normal to the surface S m at a point P m . An eﬀective r r r relative displacement λ is deﬁned by the norm of v (3.19) λ= ¯2 + ¯2 + ¯2 1 2 3 ¯ We assume that the normalized scalar traction Tv acts along the direction of v to resist the eﬀective relative displacement λ . The proposed constitutive law for the interface material is deﬁned along v, (3.20) Tv ( ¯ 1 , ¯ 2 , ¯ 3 ) = λ Q( ¯ 1 , ¯ 2 , ¯ 3 ) ¯ where Q is a decreasing function of any of the normalized relative displacements ¯ j , j = 1, 2, 3. The components of the traction acting along v, normal and tangent to the mid-surface S m at a point P m is v (3.21) ¯ ¯ r Tj = Tv ˆj · = ¯j Q v for j = 1, 2, 3. The function Q is chosen to satisfy the multi-axial stress criterion in Equation 2.1 for the onset of delamination and the mixed-mode fracture criterion in Equation 2.2 and is given by 2 − µβ /d − d ˜ ˜ (3.22) Q = exp β In the latter equation, the scalar mixed-mode parameter µ is deﬁned such that it couples the normalized relative displacements for the opening and sliding modes; i.e., ¯1 α α α 1/α (3.23) µ= + ¯2 + ¯3 where | i | is the absolute value function, and 1 = 1 if 1 > 0, otherwise it is zero. The material parameter α deﬁnes the shape of the failure surface for the onset and progression of delamination. The ˜ internal state variable d is given by, (3.24) d(ti ) = max 1, d(ti−1 ) , µβ , d(0) = 1 ˜ ˜ (t) ˜ The constitutive equations are slightly modiﬁed to take into consideration the mechanical behavior of the interface if penetration of surfaces S ± is detected. Under these contact conditions the surfaces S ± are assumed smooth so that frictional eﬀects can be neglected. When contact is formed between two smooth surfaces of adjacent lamina, the equilibrium largely depends upon the distribution of elastic forces in the contacting lamina. Adjacent lamina surfaces are under contact at a point P m , P m ∈ S m if the relative displacement 3between P ± is less than zero. For 3 < 0, a large repulsive traction T3 develops to avoid interpenetration of the surfaces S ± at P m . From Equations 3.21 to 3.24 we obtain the ﬁnal form of the mixed-mode constitutive equations as T1 ¯ 1 ¯ ¯ ¯2 2 − µβ /d − d ˜ ˜ (3.25) T2 = exp ¯ ¯ β T3 3 0 β 1+κ ¯3 + 0 exp β − −¯3 7 where κ is an interpenetration factor to magnify the repulsive force T3 , and it is chosen arbitrarily in the range κ > 1. Equations 3.25 and 3.24 reduce to Equations 3.15 and 3.16, respectively, for single-mode delamination. The empirical parameters governing the constitutive equations in 3.25 are the critical energy release rates c c c c c c GIc , GIIc , GIIIc ; the maximum interfacial strengths T1 , T2 , T3 ; the critical separation values 1, 2, 3; and the parameter β. These may be speciﬁed based on atomistic models of separation or on a phenomeno- logical basis depending whether the separation process is governed by ductile void coalescence or a brittle cleavage mechanism. By specifying the critical energy release rates and the maximum interfacial strengths, one can obtain the critical separation values. The path independent J-integral along a boundary that con- tains the interface material can be used to show that the area under the traction versus separation curve is the work of fracture per unit area. Equation 3.14 under pure Mode I, Mode II, or Mode III fracture, is used to obtain the critical separation values c , j = 1, 2, 3. j Proof. The exponential constitutive law as speciﬁed by Equations 3.24 and 3.25 satisfy Equation 2.1 for the onset of delamination, and Equation 2.2 for the progression of delamination. For simplicity, monotonically increasing loading is assumed, i.e., d = max 1, µβ . The eﬀect of inter- ˜ penetration is also neglected, 3 > 0. For the onset of delamination, the components of the traction vector ¯ in Equation 3.25 are substituted into Equation 2.1 to obtain the eﬀective traction Te as β 1/α (3.26) ¯ Te = ¯ α + ¯ α + ¯ α exp α 1 − µ 1 2 3 β 1 − µβ = µ exp β This equation is analogous to Equation 3.13 for single-mode delamination. At the initiation of delamination we set Te = 1 in Equation 3.26, to ﬁnd the only solution which is µβ = 1. Hence, the relative displacement ¯ ¯ µ = 1 at the onset of delamination when Te = 1. Therefore, the proposed constitutive law, Equation 3.25, satisﬁes Equation 2.1 for the initiation of delamination. For the progression of delamination, proportional straining is assumed. The relative displacement asso- ciated to the sliding Mode II and Mode III are written as ¯ 1 = ξ2 ¯ 3 and ¯ 2 = ξ3 ¯ 3 with ξ2 and ξ3 ﬁxed during the loading history. The terms in Equation 2.2 are evaluated as follows, ¯3 α/2 α/2 GI 0 T3 ( ¯ 1 , ¯ 2 , ¯ 3 )d ¯ 3 = ∞ GIc 0 T3 (0, 0, ¯ 3 )d ¯ 3 α/2 1 = 2/α + φ1 ( ¯ 3 ) α α (1 + ξ2 + ξ3 ) ¯1 α/2 α/2 GII 0 T1 ( ¯ 1 , ¯ 2 , ¯ 3 )d ¯ 1 = ∞ GIIc 0 T1 ( ¯ 1 , 0, 0)d ¯ 1 α/2 2 ξ2 = 2/α + φ2 ( ¯ 3 ) α α (1 + ξ2 + ξ3 ) 8 ¯2 α/2 α/2 GIII 0 T2 ( ¯ 1 , ¯ 2 , ¯ 3 )d ¯ 3 = ∞ GIIIc 0 T2 (0, ¯ 2 , 0)d ¯ 2 α/2 2 ξ3 = 2/α + φ3 ( ¯ 3 ) α α (1 + ξ2 + ξ3 ) where φj ( ¯ 3 ), j = 1, 2, 3 are exponential decaying functions with increasing ¯ 3 . The progression of delam- ination occurs when the functions φj ( ¯ 3 ) , j = 1, 2, 3 are virtually zero. Adding the last three equations shows that the power criterion in Equation 2.2 is satisﬁed. 4. Interface Finite Element. The formulation for the interface element is based on the work of Beer [21]. An iterative solution procedure is necessary because of the geometrical and material nonlinearities of the interface material. The objective of this section is to obtain the tangent stiﬀness matrix Ke and the t e internal force vector fint required in the nonlinear solution procedure. A 2n-noded isoparametric interface element with 6n degrees of freedom and applicable to three dimen- ± sional analysis is used. The element consists of an upper and lower surface Se with n-nodes each. The ± natural coordinate system is η1 and η2 . For the surfaces Se , node j has three translational degrees of free- ± ± ± dom q1j , q2j , q3j with the ﬁrst subscript implying the associated global direction. The nodal displacement vector q is arranged as follows, (4.1) q = {q+ , q− }T ± ± ± ± ± ± q± = {q11 , q21 , q31 , ..., q1n , q2n , q3n }T ± The displacement ﬁeld Uj (η1 , η2 ), j = 1, 2, 3 of the upper and lower surfaces of the element is arranged in the vector U± . The displacement vector U± is related to the global displacement degrees of freedom vector q± as, (4.2) U± = N q± where N is a 3 × 3n shape function matrix. Substituting Equation 4.2 into Equation 3.11 gives the virtual → − relative displacement vector δ in terms of δq± , − → (4.3) δ = RT N δq+ , −RT N δq− It is convenient to deﬁne the 3 × 3n matrix Bs , (4.4) Bs = RT N and the 3 × 6n relative-displacement/displacement matrix B, − → (4.5) δ = [Bs , −Bs ] δq = B δq The internal force vector of the interface element is obtained by substituting Equation 4.5 in 3.1, (4.6) e δWint = δqT m e BT T dSe = δqT fint m Se where T is the traction vector acting on the deformed mid-surface and the integration is performed over the mid-surface of the deformed element. The tangent stiﬀness matrix stems from the linearization of the internal force vector and is obtained using Taylor’s series expansion about the approximation q(i) e ∂fint (4.7) e fint (q(i) + e q) ≈ fint (q(i) ) + q + ... ∂q q=q(i) 9 where i is the iteration number. In numerical analyses, the internal force vector needs to be computed accurately, and the tangent stiﬀ- ness matrix may be computed approximately. The computation of the tangent stiﬀness matrix is intensive and a very accurate expression is not required. Therefore, the derivative of the relative-displacement ma- trix/displacement matrix with respect to the nodal displacements are neglected. In addition, the partial derivatives of M in Equation 3.12 with respect to q are neglected. Thus, from Equation 4.7, the approxi- mate 6n × 6n tangent stiﬀness matrix is (4.8) Bs = B+ = B− ˜ B = [Bs , −Bs ] ˜ where B implies approximation to B. e ∂fint (4.9) Ke = t ≈ m BT DB dSe ∂q m Se where D is the material tangent stiﬀness, and is later deﬁned in detail. Equation 4.9 is rewritten using the relation in Equation 4.8, Ks −Ks (4.10) Ke = t −Ks Ks where Ks is a 3n × 3n submatrix deﬁned as (4.11) Ks = Bs T DBs dSe m m Se The approximations for the tangent stiﬀness matrix save computational time. 4.1. Material Tangent Stiﬀness. The components of the material tangent stiﬀness D are obtained in the incremental form, ∂Ti (4.12) δTi = δ j = Dij δ j ∂ j First consider the case in which there is no interpenetration, that is, for 3 > 0. The components of D are obtained by diﬀerentiation of Equation 3.25 according to Equation 4.12, Tic ¯i¯j ¯j α−2 (4.13) Dij = c δij − Q j w µα−β ˜ ˜ where δij is the Kronecker delta, Q is given by Equation 3.22, and w is deﬁned by, (4.14) w = {1 ˜ if d = µβ d if d > µβ ˜ ˜ ˜ Now consider the case for which interpenetration is detected, that is, 3 < 0. The non-zero components of D are given by Equation 4.13 for i, j = 1, 2 and the component related to interpenetration, β β κ ¯3 (4.15) D33 = K0 1+κ ¯3 exp β c where K0 = T3 exp(1/β)/ c . The range of the values of D33 should be restricted by two conditions: (1) A 3 small D33 induces interpenetration, and (2) a large D33 produces ill-conditioned matrices. A list of references a on these restrictions is given by D´vila et al[13]. The value of D33 should be in the range, 3 3 (4.16) 106 N/mm < D33 < 107 N/mm 10 The upper bound of the condition cannot be guaranteed because of the exponential nature of Equation 4.15. Therefore, for 3 < 0, the expressions T3 and D33 are modiﬁed to have the form (4.17) T3 = K 0 3, D33 = K0 c c and K0 = T3 exp(1/β)/ 3. The material tangent stiﬀness is non-symmetric, and can be positive deﬁnite, semi-deﬁnite, or negative deﬁnite. For µ > 1, the matrix Dij is negative deﬁnite. The material tangent stiﬀness matrix has properties of an anisotropic material, one which has strong dependence on the relative displacements in all directions. For single-mode delamination, D is fully diagonal, otherwise, some of the oﬀ-diagonals are non-zero. 4.2. Consistent and Inconsistent Tangent Stiﬀness. For the full-Newton-Raphson nonlinear so- lution procedure, the consistent tangent stiﬀness matrix is used in the ﬁnite element analysis. However, when softening constitutive laws with the consistent tangent stiﬀness are employed, the tangent stiﬀness matrix is often ill-conditioned and a converged solution may not be obtained[22]. An alternative solution is to reﬁne the mesh ahead of the crack-tip or to decrease the maximum interfacial strength[15, 23]. Reﬁning the mesh size increases the computational time, and lowering the maximum interface strength can result in a premature initiation of delamination[7]. Alternatively, researchers often utilize a positive deﬁnite matrix such as the material secant stiﬀness when dealing with softening constitutive laws. However, a large number of iterations results in using the material secant stiﬀness. As an alternative, three diﬀerent modiﬁcations to the tangent stiﬀness matrix eliminate these convergence diﬃculties while a converged solution can be obtained in a small number of iterations: e e 1. Equation 4.8, Kii = max(0, Kii ), i = 1, 2, ..., 2n 2. Equation 4.9, Ksii = max(0, Ksii ), i = 1, 2, ..., n 3. Equation 4.13, Dii = max(0, Dii ), i = 1, 2, 3 The convergence rate of option 1 is better than option 2, and the convergence rate of option 2 is better than option 3. If the mesh is coarse, it is better to choose option 3. 4.3. Contact Elements. Interface elements were developed to model initial delaminated surfaces. All the components of the material tangent stiﬀness is zero, except for the case in which interpenetration is detected. If interpenetration is detected Equation 4.17 is used. Thus, these interface elements act like contact elements. 5. Finite Element Results. Numerical results are presented for quasi-static loading and unloading of the double cantilever beam (DCB), the end load split (ELS), end notch ﬂexure (ENF), and ﬁxed ratio mixed mode (FRMM) fracture test specimens. Results are also presented for quasi-static loading of the mixed mode bending (MMB). Mode I fracture occurs in the DCB, Mode II occurs in the ELS and ENF, and Mode I and II occur in the FRMM and MMB. The fracture test specimen conﬁgurations are shown in Figure 6.5. Mode I and mixed-mode test specimens are modeled with the laminate stacking sequence [0◦ ] and2 the unidirectional material properties of Graphite-Epoxy listed in Table 6.1. An isotropic material with E = E11 and ν = ν12 are used for the Mode II test specimens rather than composite. The maximum interfacial strength and the critical energy release rates are listed in Table 6.2. The geometrical properties are the length L = 100 mm, the arm thickness h = 1.5 mm, and width B = 10 mm. For the DCB, the geometrical properties are diﬀerent from the other test specimen conﬁgurations: L = 150 mm, h = 1.5 mm, and B = 20 mm. The initial crack length a0 of each test specimen is: DCB - 50 mm, ENF - 30 mm, ELS - 50 mm, FRMM - 40 mm, and MMB - 20 mm. 11 The interface elements are positioned between the upper 0◦ lamina and the lower 0◦ lamina. Delami- nation is constrained to grow in the plane between the upper and lower laminates. Interface elements with contact properties were placed along the initial crack length and interface elements formulated with the softening law are placed along the bonded length. The upper and lower laminates are modeled with C3D8I incompatible-mode 8 node solid element available in ABAQUS. Each lamina is modeled with one element through the thickness, 100 elements along the length of the laminate, and one element across the width. See Figure 6.6a. For the DCB, three elements along the width are used. The eight node isoparametric interface element for three-dimensional analysis shown in Figure 6.6b is compatible with C3D8I solid element. The element was implemented in the commercial ﬁnite element code ABAQUS as an UEL subroutine. Three point Gauss integration is used for the computation of the tangent stiﬀness matrix and internal force vector. An incremental-iterative approach is adopted for the nonlinear ﬁnite element analysis, and the Newton’s method available in ABAQUS is used to trace the loading path of the specimens with a displacement-control analysis. For the MMB, the Riks method available in ABAQUS is used. The modiﬁcation to the tangent stiﬀness matrix used is option 2 discussed in the section of interface elements. The response of the test specimens is characterized by the load-deﬂection curve. A typical ﬁnite element model of one of the test specimens consists of about 300 elements, and 2000 degrees of freedom. The computational time required was about 1200 seconds of CPU time on a Sun Solaris 2000. The average number of iterations per load increment is 7. The ﬁnite element solutions are compared to the beam analytical solutions derived from linear elastic fracture mechanics. The analytical solutions for the DCB and ENF are given by Mi et al.[15], and for the FRMM and ELS are given by Chen et al.[23]. The ﬁnite element solutions for the MMB test specimen are compared to the analytical solution in the appendix. The DCB shown in Figure 6.5a is used to determine the interlaminar fracture toughness in Mode I. The displacement w is symmetrically applied, equal and opposite at the tip of the upper and lower arm of the DCB test specimen. The corresponding reaction force P is computed. The other end of the specimen is clamped. The response of the DCB is shown in Figure 6.7a. For a loading-unloading cycle, excellent agreement of the FEM results are obtained compared to to the closed form solutions and to the experimental data([13]). The contour plot of the eﬀective von Mises stress of the DCB is shown from the top view near the delamination front in Figure 6.7b. The black strip is a region of low stress values, indicating that delamination has occurred. The gray strip is a region of intermediate stress values, and is where the material points are softening. The boundary of the black and gray strip is the location of the crack-tip. The white strip is the location of high stresses, and is the region where onset of delamination is occurring. Non-self-similar crack growth occurs because of the anticlastic bending eﬀect. The tangent stiﬀness matrix in the Newton-Raphson methods did not converge at the limit point because of the large value of the maximum interfacial strength, T c . Any of the modiﬁcations to the tangent stiﬀness matrix discussed in the section of interface elements, produced converged solutions. The ELS and ENF are shown in Figure 6.5b and 6.5c are used to determine the interlaminar fracture toughness in Mode II. For the ELS, the load P is applied at the tip such that the lower arm of the ELS remains in contact with upper arm. The other end of the specimen is clamped. The ENF specimen is simply supported, and the downward vertical displacement w2 is speciﬁed at the mid-span of the specimen. The corresponding reaction force P2 is computed. The response of the ELS and ENF are shown in Figure 6.8a and 6.8b, respectively. For a loading-unloading cycle, excellent agreement of the FEM results are obtained compared to the closed form solutions. 12 The FRMM is shown in Figure 6.5d, and is used to evaluate empirical failure criteria for mixed-mode delamination. The displacement w is speciﬁed at the tip of the upper arm and the corresponding reaction force P is computed. Mode I is 43% and Mode II is 57%. The response for α = 2 and α = 4 (see Equation 2.1 and 2.2) is shown in Figure 6.9a and 6.9b respectively. For a loading-unloading cycle, excellent agreement of the FEM results are obtained compared to the closed form solutions. The MMB is shown in Figure 6.5c, and is used to evaluate empirical failure criteria for mixed-mode delamination. The length of the lever arm c described in the report by Reeder[20] is chosen such that the mixed mode ratio from pure Mode I to pure Mode II can be varied. In this paper, c = 43.72 mm, so that the Mode I and Mode II contributions are 50% each. The MMB is simply supported, and two proportional loads are applied. The load P1 is applied upward at the tip of the upper arm, and another load P2 is applied downward at the mid-span. During the loading, the ratio P1 /P2 = 2c/(2c + L) is ﬁxed. The responses for α = 4 and α = 2 are shown in Figure 6.10a and 6.10b. The ﬁnite element response is compared to the analytical solutions in the appendix. In the ﬁrst analysis, geometric nonlinearity is used. In the second analysis both geometric linearity and nonlinearity are compared with the analytical solutions. The discrepancies on the response corresponding to the stable crack growth of the load-deﬂection response are because the analytical solution does not consider the eﬀects of geometric nonlinearities. Excellent agreement is obtained with the analytical solutions. 6. Concluding Remarks. The mechanics of an idealized interface material is presented. The kinemat- ical relations and the irreversible constitutive law mathematically describe the mechanics of the delamination process. The delamination process comprises three interrelated phases: the initiation of delamination, the evolution of the degradation zone, and the delamination growth. It predicts initiation of delamination based on a multi-axial stress criterion, and progression of delamination based on an empirical mixed-mode fracture criterion. A damage parameter is included to prevent the restoration of the previous cohesive state between the interfacial surfaces. The constitutive law is implemented with interface elements using the principal of virtual work. To demonstrate the irreversibility capability of the constitutive law, steady-state crack growth is simulated for quasi-static loading-unloading cycle of various fracture test specimen conﬁgurations. The ﬁnite element solutions are in excellent agreement with the analytical solutions. REFERENCES [1] E. F. Rybicki and M. F. Kanninen, A Finite Element Calculation of Stress Intensity Factors by a Modiﬁed Crack Closure Integral. Eng. Fracture Mech., 9, pages 931–938, 1977. [2] I. S. Raju, Calculation of Strain-Energy Release Rates with Higher Order and Singular Finite Elements. Eng. Fracture Mech, 28, pages 251–274, 1987. [3] D. S. Dugdale, Yielding of Steel Sheets Containing Clits. J. Mech. Phys. Solids, 8, pages 100–104, 1960. [4] G. I. Barrenblatt, The Mathematical Theory of Equilibrium of Cracks in Brittle Fracture. Adv. Appl. Mech., 9, pages 55–129, 1962. [5] A. Hilleborg, M. Modeer, and I.E. Petersson, Analysis of Crack Formation and Crack Growth in Concrete by Means of Fracture Mechanics and Finite Elements. Cement & Concrete Res., 6, pages 773–782, 1976. [6] A. Needleman, A Continuum Model for Void Nucleation by Inclusion Debonding. J. Appl. Mech., 54, pages 525–531, 1987. 13 [7] V. K. Goyal-Singhal and E.R. Johnson, Computational Issues in Modeling the Delamination Process using Interface Finite Elements. In Proceedings of the American Society for Composites, 16th Technical Conference, (9-12 September 2001, Blacksburg, VA) Technomic Publishing Co., Inc., Lancaster, PA, CD-ROM, 2001. [8] J. H. Rose, J. Ferrante, and R. J. Smith, Universal Binding Energy Curves for Metals and Bimetallic Interfaces. Physical Review Letters, 47(9), pages 675–678, 1981. [9] X. Xu and A. Needleman, Numerical Simulations of Fast Crack Growth in Brittle Solids. J. Mech. Phys. Solids, 42, pages 1397–1434, 1994. [10] K. W. Shahwan and A. M. Waas, Non-self similar Decohesion along a Finite Interface of Unilaterally Constrained Delaminations. Proc. R. Soc. Lond. A., 153, 197, pages 515–550, 1997. [11] M. Ortiz and A. Pandolfi, Finite-Deformation Irreversible Cohesive Elements for Three- Dimensional Crack-Propagation Analysis. Int. J. Numer. Meth. Eng., 44:1267–1282, 1999. [12] S. Mohammadi, D.R.J. Orwen, and D. Peric, A Combined Finite/Discrete Element Algorithm for Delamination Analysis of Composites. Finite Element in Analysis and Design, 28(4), pages 321–336, 1998. [13] C. G. Davila, P. Camanho, and M.F.S.F. de Moura, Mixed-Mode Decohesion Elements for ´ Analyses of Progressive Delamination. In Proceedings of the 42nd AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics and Materials Conference, Seattle, Washington, April 16-19, 2001. [14] O. Allix and P. Ladeveze, Interlaminar Interface Modelling for the Prediction of Delamination. ` Composite Structures, 22, pages 235–242, 1992. [15] Y. Mi, M. A. Crisfield, G.A.O. Davies, and H.-B. Hellweg, Progressive Delamination Using Interface Elements. Journal of Composite Materials, 32, pages 1246–1273, 1998. [16] M. de Moura, J. A. Marques, and P. de Castro, Modeling Compression Failure after Low Velocity Impact on Laminated Composites using Interface Elements. Journal of Composite Materials, 31(15), pages 1462–1479, 1997. [17] C. G. Davila and P. Camanho, Decohesion Elements using Two and Three-Parameter Mixed-Mode ´ Criteria. In American Helicopter Society International Structures Specialists’ Meeting, Williams- burg, VA, October 30-November 1, 2001. [18] J. D. Whitcomb, Analysis of Instability-Related Growth of a Through-Width Delamination. NASA TM 86301, 1984. [19] E. M. Wu and R. C. Reuter Jr., Crack Extension in Fibreglass Reinforced Plastics. Report No. 275, T & AM, University of Illinois, 1965. [20] J. R. Reeder, An Evaluation of Mixed-Mode Delamination Failure Criteria. NASA Technical Memo- randum 104210, February 1992. [21] G. Beer, An Isoparametric Joint/Interface Element for the Finite Element Analysis. Int. J. Numer. Methods Eng., 21, pages 585–600, 1985. [22] Rene de Borst and J. G. Rots, Occurrence of Spurious Mechanisms in Computations of Strain- ´ Softening Solids. Eng. Comput., 6, pages 272–280, 1989. [23] J. Chen, M. A. Crisfield, A. J. Kinloch, E. P. Busso, F. L. Matthews, and Y. Qiu, Predicting Progressive Delamination of Composite Material Specimens Via Interface Elements. Mechanics of Composite Materials and Structures, 6, pages 301–317, 1999. 14 Table 6.1 Graphite-Epoxy Properties E11 E22 , E33 G12 , G13 G23 ν12 , ν13 ν23 150 GPa 11.0 GPa 6.0 GPa 3.7 GPa 0.25 0.45 Table 6.2 Interface Material Properties c c c T2 ,T3 T1 GIc , GIIc GIIIc 10.5 ksi 9.0 Ksi 1.31 lb/in. 3.30 lb/in. S+ xi+ (η1,η2) Ui + (η1,η2) S0 Xi (η1,η2) X3, x3, U3 U± xi− (η1,η2) Ui − (η1,η2) S− X2, x2, U2 Undeformed Deformed X1, x1, U1 Configuration Configuration Fig. 6.1. Interface material deformation. D3, T3 P+ S+ ˆ r3 D2, T2 ˆ r2 Pm D1, T1 Pm ˆ r1 Sm x3 P− S− x2 x1 Fig. 6.2. Interface material mid-surface. 15 1 0.8 0.6 c T /T b =1 0.4 b = 2.2 0.2 b = 5.4 0 0 1 2 3 4 5 ∆ / ∆c Fig. 6.3. Traction-stretching curve of spring as a function of β 3 1 2 T /T c 4, 6 5 1 1 ∆ / ∆c Fig. 6.4. Traction-stretching curve as a function of the evolution of damage of the spring with β = 1 16 P, w a0 a0 h h L L P, w P, w (a) Mode I – DCB (b) Mode II – ELS P2, w2 P1, w1 P, w a0 a0 h h L L (c) Mode II – ENF, P1 = 0 (d) Mixed-Mode – FRMM Mixed-Mode – MMB, P1 ≠ 0 Fig. 6.5. Fracture test specimen conﬁgurations. 4 1 3 Upper i3 P2, w2 Upper surface 2 i2, η2 laminate Integration i1, η1 Interface Lower point 8 elements laminate Mid-surface 7 5 Lower 6 surface (a) Finite element model of the ENF (b) Eight-node isoparametric interface element Fig. 6.6. Finite element modeling. 17 70 60 1 50 Reaction Delaminated force, 40 3 2 P (N) 30 20 FEM, Present Crack front Free 10 Experiment Direction of edge Analytical, Mi et al., 1998 0 crack growth 0 3 6 9 12 15 18 Opening displacement, 2w (mm) (a) Load-opening response of the DCB (b) Non-self similar delamination growth Fig. 6.7. DCB with a0 = 50mm 120 400 320 90 Reaction Reaction 240 force, 60 force, P (N) P 2 (N) 160 30 FEM Loading-Unloading 80 FEM Loading FEM, Present Analytical, Chen, et al., 1999 Analytical, Mi, et al., 1998 0 0 0 6 12 18 24 30 0 1.5 3 4.5 6 7.5 9 Applied displacement, w (mm) Mid-span displacement, w 2 (mm) (a) ELS with a0 =50 mm (b) ENF with a0 =30 Fig. 6.8. Load-displacement response of Mode II test specimen conﬁgurations. 18 60 60 50 50 40 40 Reaction Reaction force, 30 force, 30 P (N) P (N) 20 20 10 10 FEM Linear FEM Quadratic Analytical, Linear, Chen, et al., 1999 Analytical, Quadratic, Chen, et al.,1999 0 0 0 5 10 15 20 25 30 0 5 10 15 20 25 30 Tip displacement, w (mm) Tip displacement, w (mm) (a) FRMM with α=2 and a0 =40 mm (b) FRMM with α=4 and a0 =40 mm Fig. 6.9. Load-displacement response of the FRMM test specimen conﬁgurations. 125 120 100 100 80 75 Reaction Reaction force force, 60 P 1, (N) 50 P 1 (N) 40 FEM, Geometrically Nonlinear 25 20 FEM, Quadratic FEM, Geometrically Linear Analytical, Quadratic, Appendix Analytical, Appendix 0 0 0 2 4 6 8 10 0 2 4 6 8 10 Applied displacement, w 1 (mm) Applied displacement, w 1 (mm) (a) MMB with α=4 and a0 =20 mm (b) MMB with α=2 and a0 =20 mm Fig. 6.10. Load-displacement response of the MMB test specimen conﬁgurations. 19 Appendix A. Mixed-Mode Analytical Solutions. The beam analytical solutions based on linear elastic fracture mechanics for the MMB test specimen are presented without details. In general, the total energy release rate is (A.1) GT = GI + GII GI and GII are the Mode I and Mode II energy release rate contributions. The delamination propagates when, (A.2) GT = G c = G m + G m I II and Gc is the critical energy release rate, Gm and Gm are the the Mode I and Mode II energy release rates I II at crack propagation. For all the fracture test specimens, it is possible to express φ = Gm /Gm , where I II φ ∈ [0, ∞), so that the Gc value can be computed based on the fracture criterion in Equation 2.2 α/2 (α/2) −(2/α) φ 1 (A.3) Gc = (1 + φ) + GIc GIIc The derivations to obtain the expression of φ for the MMB specimen are omitted here, and is GI Gm I 4 6c − L (A.4) φ= = m = GII GII 3 2c + L where c is the length of the lever arm in the test ﬁxture ([20]), and L is the length of the MMB specimen. For simplifying purposes, the loads PI and PII associated to modes I and II respectively are deﬁned as L 6c − L L 2c + L (A.5) PI = P1 , PII = P1 c 4L c L The load P1 is deﬁned in Figure 6.5c. The initial load-deﬂection response is linear and given by 16L 6c − L P1 a3 0 (A.6) w1 = 3c 4L EI where E is the Young’s Modulus and I is the moment of inertia. The load-deﬂection response, when delamination propagates with a < L/2 is 3/2 16PI 8BEIGc (A.7) w1 = 2 2 3EI 64PI + 3PII where B is the width of the beam. The load-displecement relation when delamination propagates with a > L/2 is obtained by solving the quadratic equation for a, (A.8) 2 2 64PI + 3PII − 64PI PII a2 2 2 − 6PII L − 32PI PII L a + 3PII L2 − 8BEIGc = 0 and substituting its solution into 16L 6c − L P1 a3 (A.9) w1 = 3c 4L EI 20 Form Approved REPORT DOCUMENTATION PAGE OMB No. 0704-0188 Public reporting burden for this collection of information is estimated to average 1 hour per response, including the time for reviewing instructions, searching existing data sources, gathering and maintaining the data needed, and completing and reviewing the collection of information. Send comments regarding this burden estimate or any other aspect of this collection of information, including suggestions for reducing this burden, to Washington Headquarters Services, Directorate for Information Operations and Reports, 1215 Je erson Davis Highway, Suite 1204, Arlington, VA 22202-4302, and to the O ce of Management and Budget, Paperwork Reduction Project 0704-0188, Washington, DC 20503. 1. AGENCY USE ONLYLeave blank 2. REPORT DATE 3. REPORT TYPE AND DATES COVERED August 2002 Contractor Report 4. TITLE AND SUBTITLE 5. FUNDING NUMBERS AN IRREVERSIBLE CONSTITUTIVE LAW FOR MODELING THE DELAMINATION PROCESS USING INTERFACE ELEMENTS C NAS1-97046 WU 505-90-52-01 6. AUTHORS a Vinay K. Goyal, Eric R. Johnson, Carlos G. D vila, and Navin Jaunky 7. PERFORMING ORGANIZATION NAMES AND ADDRESSES 8. PERFORMING ORGANIZATION ICASE REPORT NUMBER Mail Stop 132C ICASE Report No. 2002-25 NASA Langley Research Center Hampton, VA 23681-2199 9. SPONSORING MONITORING AGENCY NAMES AND ADDRESSES 10. SPONSORING MONITORING National Aeronautics and Space Administration AGENCY REPORT NUMBER Langley Research Center NASA CR-2002-211758 Hampton, VA 23681-2199 ICASE Report No. 2002-25 11. SUPPLEMENTARY NOTES Langley Technical Monitor: Dennis M. Bushnell Final Report To be submitted to Composite Structures. 12a. DISTRIBUTION AVAILABILITY STATEMENT 12b. DISTRIBUTION CODE Unclassi ed Unlimited Subject Category 34 Distribution: Nonstandard Availability: NASA-CASI 301 621-0390 13. ABSTRACT Maximum 200 words An irreversible constitutive law is postulated for the formulation of interface elements to predict initiation and progression of delamination in composite structures. An exponential function is used for the constitutive law such that it satis es a multi-axial stress criterion for the onset of delamination, and satis es a mixed mode fracture criterion for the progression of delamination. A damage parameter is included to prevent the restoration of the previous cohesive state between the interfacial surfaces. To demonstrate the irreversibility capability of the constitutive law, steady-state crack growth is simulated for quasi-static loading-unloading cycle of various fracture test specimens. 14. SUBJECT TERMS 15. NUMBER OF PAGES composite structures, progressive failure, ply damage mode, intradamage mode, 25 interlaminar damage mode, delamination, interface elements, decohesion elements, 16. PRICE CODE buckling, postbuckling A03 17. SECURITY CLASSIFICATION 18. SECURITY CLASSIFICATION 19. SECURITY CLASSIFICATION 20. LIMITATION OF REPORT OF THIS PAGE OF ABSTRACT OF ABSTRACT Unclassi ed Unclassi ed NSN 7540-01-280-5500 Standard Form 298Rev. 2-89 Prescribed by ANSI Std. Z39-18 298-102